DRAFT SF 298 - Defense Technical Information · PDF fileDRAFT SF 298 1. Rkeport Date ... The...
Embed Size (px)
Transcript of DRAFT SF 298 - Defense Technical Information · PDF fileDRAFT SF 298 1. Rkeport Date ... The...
DRAFT SF 2981. Rkeport Date (dd-mm-yy) 2. Report Type 3. Dates covered (from... to)
4. Title & subtitle 5a. Contract or Grant #Effects of Alloy Chemistry Changes on SacrificialAluminum Anode Performance
Tri-Service Committee on Corrosion Proceedings5b. Program Element #
6. Author(s) 5c. Project #Dr. John N. MurrayMr. Richard A. Hays 5d. Task #Mr. Douglas W. Smith
5e. Work Unit#
7. Performing Organization Name & Address 8. Performing Organization Report #
9. Sponsoring/Monitoring Agency Name & Address 10. Monitor AcronymTri-Service Committee on CorrosionUSAF WRIGHT-PATTERSON Air Force Base, Ohio 45433 11. Monitor Report #
12. Distribution/Availability StatementApproved for Public ReleaseDistribution Unlimited
13. Supplementary Notes
15. Subject TermsTri-Service Conference on Corrosion
A PON ... i 19. Limitation 20. # of 21. Responsible Person................................. of Abstract Pages (Name and Telephone #)
16. Report 17. Abstract 18. This Page
21-23 JUNE 1994
SHERATON PLAZA HOTELORLANDO, FLORIDA
Effects of Alloy Chemistry Changeson Sacrificial Aluminum Anode Performance
Dr. John N. Murray*, Mr. Richard A. Haysand Mr. Douglas W. Smith
Carderock Division, Naval Surface Warfare Center, (CDNSWC)
Marine Corrosion Branch, Code 6133A Leggett Circle
Annapolis, MD 21402
The set of aluminum alloy sacrificial anodes taken from theupper starboard stern array from a Navy submarine was evaluated atCDNSWC to determine the cause of non-uniform utilization duringthe approximately 30 month anode service period. Physical datafrom the used anodes as well as electrochemical characterizationswere determined. The evidence indicated that the three distinctlevels of anode weight change (and estimated discharge current)could be attributed to distinct levels of mercury contamination inthe three heats of alloy from which these particular anodes weretaken. The experience shows that reasonable vendor care in alloypreparation and anode casting must be taken for uniform anodeperformance to be achieved in multi-anode array applications.
A US Navy submarine was outfitted with a ship set of Galvalum.III, indium activated, aluminum alloy sacrificial anodes duringthe February 1990 post shakedown availability. The anodes hadbeen procured by the Electric Boat (EB) Division of General :2Dynamics using an EB purchase specification. The EB purchasespecification was modeled on a CDNSWC draft version of a militaryspecification (Draft MIL-SPEC), "Anodes, sacrificial, aluminumalloy,,. Anodes from essentially all heats of the procurement wereselected by the EB inspectors, shipped to CDNSWC and subjected to
the QA/QC procedures by CDNSWC as outlined in the EB purchaseSpecification. In general, the electrochemical performance of theanode heats was found to be acceptable. However, Heat 3069 was
The anode installations and various outfitted tanks and spaces were rein-
spected in early October 1992. In general. the anode consumption rates were foundto be as expected for the approximately 30 months of service exposure. The tanksand voids were also found to be protected with little paint deterioration or metalcorrosion which might be attributed to improper anode installation or inadequateanode performance. However. there was a rather marked non-uniform anodeconsumption which was observed on each of the four stem array anode strings.A typical view of the first 11 of the 21 AHC- 10 anodes from the upper starboardarray is shown as Figure 1. Counting from forward to aft. anodes 2, 3, 7 and 11appeared to be essentially unused. On-site visual estimnates of 40-60% al' ),, con-sumption of the majority of the anodes v crc made. Simple o- site checks of themountiu,-bolt-to-alloy-bodv electrical continuity showed all anodes of the upperstring were electrically connected to the hull. Although there were only 17 of 84anodes on the stem which had this "unused" appearance. the behavior was ofsufficient concern to warrant a low level investigation as to cause. It should benoted that the 67 "good" anodes would be sufficient for cathodic protection ofthe stern. One possible assumption of cause of anode non-use was that these 17anodes were "dead". that is, the surface oxide coating which had formed duringthe 6 months following fabrication and before wetting in the estuary waters wassufficiently tenacious that the pieces were comuletely passivated. ie.. inactive.
Figure 1. Upper stem aluminum alloy array, 688 Class. 30 months service.
If one makes hat assumption, then removing and evaluating the anodes from thearray after they became exposed in the dry dock environment carries the risk ofdifferent reactivations in the subsequent laboratory test environment. This mightsuggest the laboratory test results would not relate to the anode status just prior todrydocking. In addition, the submarine sat pierside for an undisclosed periodprior to drydocking, during which time metal ion impurities (such as copper fromthe anti-fouling coating system) could have electrodeposited on the sacrificialanode surfaces affecting the general electrochemical performance characteristics.With at least these two caveats, as the stern arrays were to be replaced with newaluminum anodes, a decision was made to mark and return the upper stern arrayto CDNSWC for further analysis. The initial effort was to be limited to weighingthe anodc6 and simple electrochemical testing.
Therefore, the overall objective of this effort was to attempt to determine ifthe cause of non-uniform anode consumption could be identified This papersummarizes the effort and findings of the study.
The anodes were purchased by EB in accordance with the EB material specifi-cation. Material chemistry and electrochemical performance data of samples takenfrom unused anodes from all of the heats were determined previously and selectedvalues are included later in the Results and Discussion section.
The tagged, 6 x 12 x 1.25", AHC-10 anodes from "ie upper starboard stemrarray were received at CDNSWC, weighed in the as-received condition, nylonbrush cleaned under flowing water, dried overnight at ambient conditions andreweighed. The heat numbers of many of the anodes were still legible on the"backside" of the anodes and these were noted. Physical dimensions of eachanode were also recorded.
Two types of electrochemical tests were performed. The full sized, cleanedanodes were positioned vertically in a 12" x 12" x 12" polyethylene tank. Acarbon steel plate counterelectrode was positioned approximately 7 inches fromand parallel with the test anode. The electrochemical reactivating cliaracteristicsWere determined by monitoring the anode potential for roughly a one day periodWhile discharging the test anode at a constant current of 288 mA. This currentwas selected as approximating the discharge current density of 4 mA/in2 used inthe previous smaller sample QA/QC test effort. The 288 mA current assumesonly the alloy surface facing the counterelectrode contributed appreciably to thedischarge process.
All testing was performed at laboratory ambient temperature (20-23C,68-75F) using aerated ASTM-D-1141, substitute ocean water. The electrolytebath was not changed until after testing three anodes, as the small amount ofaccumulated anode reaction products was judged not to be affecting the electro-chemical performance.
Three anodes, selected as typical for each observed type of repassivationbehavior, were tested further. Two preselected pairs from these three anodes weresubjected to an overnight galvanic couple experiment, followed by full potentio-dynamic scans in the range of - 1200 to - 700 mV. vs. saturated calomel referenceelectrode (SCE). Several additional runs were made with new zinc and newGalvalum III anodes as well as used zinc and estuary-exposed Galvalum IIIpieces. After the test electroly- was contaminated vith zinc anode r-actionproducts, another zinc anode was tested or the test cell was replenished withfresh test solution.
RESULTS AND DISCUSSION
The weights of the cleaned anodes are summarized in Table 1 by tag numberwhich should correspond to the linear position coming aft in the upper starboardstem array. The anode tag numbers of the four anodes which showed little con-sumption do not quite agree with the photographic data and notes from theinspection but the tag numbers will be utilized throughout the rest of this report.Subtracting the used anode weight from the 3951 gram alloy average initialweight as well as the 272 gram steel strap weight determined previously for theAHC-10 anodes (and correcting for the machined leading and lagging taper ofthe two end anodes), results in the approximate weight change values shown inTable I for the anodes during the approximately 30 month exposure. The weightchange values were converted to averaged anode currents utilizing 90% averagedFaradaic efficiencies determined previously. The calculated current data are thensummarized as Figure 2. A column of percentage used (or percentage consumed)is included in Table 1. As the actual values of the "active" anodes ranged from15 to 35%, the availability of a set of comparative visual standards would prob-ably have resulted in better estimates than the 40-60% range made during thedrydock inspection.
Table 1Anode Weights Calculated Weight Changes and Anode Currents
Anode Cleaned Calculated Percent Calculated (mA) HeatNumber Weight (2_) Weight loss (Lg Used Anode Current Number1 3061.1 1095 28 134 *31602 2924.9 1298 32 159 30703 4042.0 181 - 5 22 30694 4122.0 101 3 12 -- 695 2811.5 141